#------------------------------------------------------------------------------
#$Date: 2015-01-27 21:58:39 +0200 (Tue, 27 Jan 2015) $
#$Revision: 130149 $
#$URL: svn://www.crystallography.net/cod/cif/4/00/06/4000661.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4000661
_journal_name_full               'Chemistry of Materials'
_journal_paper_doi               10.1021/cm0518067
_journal_year                    2005
_chemical_formula_sum            'Ge Mn Te4 Tl2'
_chemical_formula_weight         1046.67
_chemical_name_common            'Thallium Manganese Germanium Telluride'
_space_group_IT_number           121
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  'I -4 2'
_symmetry_space_group_name_H-M   'I -4 2 m'
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   8.399(3)
_cell_length_b                   8.399(3)
_cell_length_c                   6.963(3)
_cell_measurement_temperature    175(5)
_cell_volume                     491.2(3)
_diffrn_ambient_temperature      175(5)
_exptl_crystal_density_diffrn    7.077
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Tetragonal' changed to 'tetragonal'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_database_code               4000661
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'y, -x, -z'
'-y, x, -z'
'-x, y, -z'
'x, -y, -z'
'-y, -x, z'
'y, x, z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-y+1/2, x+1/2, -z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-y+1/2, -x+1/2, z+1/2'
'y+1/2, x+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Tl1 Tl 0.0000 0.5000 0.0000 0.01901(16) Uani 1 4 d S . .
Mn1 Mn 0.0000 0.0000 0.5000 0.0151(9) Uani 1 8 d S . .
Ge1 Ge 0.0000 0.0000 0.0000 0.0077(5) Uani 1 8 d S . .
Te1 Te 0.17288(6) 0.17288(6) 0.23160(9) 0.00927(16) Uani 1 2 d S . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Tl1 Tl1 3.4815(13) 11_455 ?
Tl1 Tl1 3.4815(13) 11_454 ?
Tl1 Te1 3.5011(10) 4 ?
Tl1 Te1 3.5011(10) 3_565 ?
Tl1 Te1 3.5011(10) 2_565 ?
Tl1 Te1 3.5011(10) . ?
Tl1 Te1 3.6262(10) 12 ?
Tl1 Te1 3.6262(10) 11_455 ?
Tl1 Te1 3.6262(10) 9_454 ?
Tl1 Te1 3.6262(10) 10_554 ?
Tl1 Ge1 4.1995(14) . ?
Tl1 Ge1 4.1995(14) 1_565 ?
Mn1 Te1 2.7765(9) 2 ?
Mn1 Te1 2.7765(9) . ?
Mn1 Te1 2.7765(9) 4_556 ?
Mn1 Te1 2.7765(9) 3_556 ?
Mn1 Tl1 4.1995(14) 9_545 ?
Mn1 Tl1 4.1995(14) 11_455 ?
Mn1 Tl1 4.1995(14) 9_445 ?
Mn1 Tl1 4.1995(14) 11_445 ?
Ge1 Te1 2.6110(9) . ?
Ge1 Te1 2.6110(9) 4 ?
Ge1 Te1 2.6110(9) 3 ?
Ge1 Te1 2.6110(9) 2 ?
Ge1 Tl1 4.1995(14) 3 ?
Ge1 Tl1 4.1995(14) 3_455 ?
Ge1 Tl1 4.1995(14) 1_545 ?
Te1 Tl1 3.5011(10) 3 ?
Te1 Tl1 3.6262(10) 11_455 ?
Te1 Tl1 3.6262(10) 9_545 ?
